# On the stress–force–fabric relationship for granular materials

18

(1)

## On the stress–force–fabric relationship for granular materials

a,b,⇑

### , H.-S. Yu

b a

Process and Environmental Research Division, Faculty of Engineering, The University of Nottingham, University Park, Nottingham NG7 2RD, UK b

Materials, Mechanics and Structures Research Division, Faculty of Engineering, The University of Nottingham, University Park, Nottingham NG7 2RD, UK

### i n f o

Article history:

Received in revised form 12 December 2012 Available online 17 January 2013 Keywords:

Stress–force–fabric (SFF) relationship Directional statistics

Anisotropy

Multi-scale investigations Discrete element method (DEM)

### a b s t r a c t

This paper employed the theory of directional statistics to study the stress state of granular materials from the particle scale. The work was inspired by the stress–force–fabric relationship proposed by Roth-enburg and Bathurst (1989), which represents a fundamental effort to establish analytical macro–micro relationship in granular mechanics. The micro-structural expression of the stress tensor

ij¼1V

P

c2V

### v

cifjc, wherefc

i is the contact force and

### v

ciis the contact vector, was transformed into directional integration by grouping the terms with respect to their contact normal directions. The directional statistical theory was then employed to investigate the statistical features of contact vectors and contact forces. By approximat-ing the directional distributions of contact normal density, mean contact force and mean contact vector with polynomial expansions in unit direction vectorn, the directional dependences were characterized by the coefﬁcients of the polynomial functions, i.e., the direction tensors. With such approximations, the directional integration was achieved by means of tensor multiplication, leading to an explicit expres-sion of the stress tensor in terms of the direction tensors. Following the terminology used inRothenburg and Bathurst (1989), the expression was referred to as the stress–force–fabric (SFF) relationship.

Directional statistical analyses were carried out based on the particle-scale information obtained from discrete element simulations. The result demonstrated a small but isotropic statistical dependence between contact forces and contact vectors. It has also been shown that the directional distributions of contact normal density, mean contact forces and mean contact vectors can be approximated sufﬁciently by polynomial expansions in directionnup to 2nd, 3rd and 1st ranks, respectively. By incorporating these observations and revoking the symmetry of the Cauchy stress tensor, the stress–force–fabric relationship was further simpliﬁed, while its capacity of providing nearly identical predictions of the stresses was maintained. The derived SFF relationship predicts the complete stress information, including the mean normal stress, the deviatoric stress ratio as well as the principal stress directions.

The main beneﬁts of deriving the stress–force–fabric relationship based on the directional statistical theory are: (1) the method does not involve space subdivision and does not require a large number of directional data; (2) the statistical and directional characteristics of particle-scale directional data can be systematically investigated; (3) the directional integration can be converted into and achieved by ten-sor multiplication, an attractive feature to conduct computer program aided analyses.

1. Introduction

Granular materials often exhibit sophisticated collective behav-ior even though they consist of solid particles with relatively

sim-ple particle–particle interactions. This makes multi-scale

investigation an important branch of granular mechanics. Parti-cle-scale information, which was a difﬁcult and rare source to ob-tain in history, has nowadays become easily accessible, mainly due to the emergence and fast growth of the discrete element method

(DEM) (Cundall and Strack, 1979). The good qualitative agreement between laboratory observations and DEM simulations has made DEM a popular numerical tool for multi-scale investigations. One of the remaining challenges, as addressed in the current paper, is to extract the key statistical features from the massive amount of particle-scale information in order to advance our understanding in granular materials.

The micro-structural deﬁnition of the stress tensor is a well-established starting point of many multi-scale investigations. In case of static equilibrium, the stresses acting on the material boundary are transmitted through the internal structure and in equilibrium with the inter-particle interactions. Viewing a granu-lar material as an assembly of granugranu-lar particles with only point

⇑ Corresponding author at: Process and Environmental Research Division, Faculty of Engineering, University Park, The University of Nottingham, Nottingham NG7 2RD, UK. Tel.: +44 1159514167; fax: +44 1159513898.

Contents lists available atSciVerse ScienceDirect

## International Journal of Solids and Structures

(2)

contact, the macro stress tensor could be evaluated from the tensor product of contact forcesfc

i and contact vectors

ci as:

¼1 V

X

c2V

c

if

c

j ð1Þ

in which

### r

ijstands for the average stress tensor over volumeV. To be consistent with the sign convention in soil mechanics, a contact vector is deﬁned as the vector pointing from the contact point to the particle centre. Eq.(1)links the stress tensor deﬁned at equivalent continuum scale with inter-particle contact forces (Love, 1927; We-ber, 1966; Goddard, 1977; Christoffersen et al., 1981; Rothenburg and Selvadurai, 1981; Bagi, 1996; Li et al., 2009). It has been derived rigorously for quasi-static granular materials based on the Newton’s 2nd law of motion with only the uniformity and point contact assumption.

Like many other relationships addressing homogenization be-tween macro and micro variables, the expression of Eq.(1)involves summation over a massive amount of particle-scale information as appeared on the right hand side of the equation. It is a source of complication pertinent to the fact that the particle-scale information, including both contact vectors and contact forces, are random variables, and intrinsically direction dependent (Drescher and De Josselin de Jong, 1972; Oda et al., 1982; Cundall and Strack, 1983).

The development and application of the statistical theory to

process directional data has been pioneered byKanatani (1984).

His work dealt with unit vectors. Examples in the context of gran-ular mechanics are contact normals and particle orientations. Being aware that the physical quantities, like forces, displace-ments, are to be represented by vectors, reﬂecting information on both their directions and magnitudes,Li and Yu (2011)have ex-tended the mathematical formulations (Kanatani, 1984) to vector-valued directional data. The form of polynomial expansions in

directionnhas been followed to approximate the directional

dis-tributions. And the least square error criterion has been employed to determine the tensorial coefﬁcients, i.e., the direction tensors. These direction tensors are macroscopic measures deﬁned on the statistics of particle-scale directional data. They can be used as macro variables for the development of the micro–macro relation-ships and physical laws reﬂecting fundamental mechanisms. The theoretical formulations and the applied techniques have been published in a preceding paper (Li and Yu, 2011).

Directional statistical analyses are of particular importance in the study of material anisotropy, which has been recognized as an important aspect of granular material behaviors for many years

(Casagrande and Carrillo, 1944; Drescher and Josselin De Jong,

1972; Oda, 1972; Oda et al., 1985). Rothenburg and Selvadurai

(1981) were among the ﬁrst to introduce Fourier series in the

description of the directional dependence of contact normal den-sity. Such an approximation has been shown to have the root in

the directional statistical theory (Kanatani, 1984). Rothenburg

and Bathurst (1989)also used Fourier series to approximate the

directional distributions of mean normal contact force and mean tangential contact force with coefﬁcients interpretable as mea-sures of anisotropy in respective quantities. They hence derived the stress–force–fabric (SFF) relationship for two dimensional assemblies consisting of disks, and later extended the expression

to two dimensional elliptical-shaped particles (Rothenburg and

Bathurst, 1993) and three dimensional ellipsoidal particles with

anisotropy tensors (Ouadfel and Rothenburg, 2001).

The SFF relationship proposed by Rothenberg and his co-work-ers formulated the macroscopic stress tensor as an explicit statisti-cal description in terms of anisotropic parameters. It provides a micromechanical insight into the continuum-scale shear strength of granular materials. However, the basic assumptions made

during their derivation have not been fully validated, mainly: (i) the contact vectors and the contact forces in each direction are sta-tistically independent; (ii) the Fourier functions up to 2nd rank are sufﬁcient to approximate the directional distributions of contact normal density, normal and tangential contact forces.

The main objective of this paper is to apply the mathematical theory of directional statistics to conduct the multi-scale investiga-tion on the stress state of granular materials. In particular, we will revisit and study the validity of the key assumptions made by Rothenberg and his co-workers with the newly developed direc-tional statistical theory. In this paper, unless indicated otherwise an Einstein summation convention is adopted for repeated subscripts.

2. General form of the stress–force–fabric relationship

2.1. Integral form of the micro-structural stress tensor

Let X represent the unit circle in two dimensional spaces

(D¼2) or the unit sphere in three dimensional spaces (D¼3).

We denote the total number of contacts in a granular assembly asM, andDMðnÞrepresents the number of contacts whose normal directions fall into the stereo-angle elementDXcentered at direc-tionn. The terms on the right hand side of Eq.(1)can be grouped according to their contact normal directions, leading to:

¼1 V

X

X

h

ifjijn

MðnÞ ¼

M V

X

X ecðnÞh

ifjijn

### DX

ð2Þ

where⁄|ndenotes the value of variable⁄in directionn, andh⁄i|n denotes the average value of all terms of⁄sharing the same contact normal directionn. The discrete spectra of functionecðnÞ ¼DMðnÞ= DXis the probability density of contact normals. ec(n)DX repre-sents the probability that an arbitrary selected contact has a normal direction falling within the stereo-angle elementDX. When the

ste-reo-angle increment approaches zero, we have ecðnÞ ¼lim

DX!0 DMðnÞ=DX. It becomes a continuous function at the thermodynamic limit.

The average number of contacts per particle is

### x

=M/N, where

Nis the total number of particles. In the case of thermodynamic

limit,

### x

approaches a limit, i.e., lim

N!1M=N¼

### x

. It is referred to as the coordination number, an index characterizing the packing den-sity. WhenDX!0, transition leads to an expression of the stress tensor in terms of integration over all stereo-angles as:

¼

N V

I

X ecðnÞh

ifjijnd

### X

ð3Þ

wheredXis an elementary solid angle.

Eq.(3)involves the joint producth

### v

ifji|nwithin the integration. In general,h

ifji|n–h

### v

ii|nhfji|n, where h

### v

ii|n and hfji|n denote the mean contact vector and the mean contact force along direction

nrespectively. For randomly distributed contact vectors

### v

and con-tact forcesf, the covariance matrix:

Covð

jn;fjnÞ ¼ ð

jn h

ijnÞ ðfjn hfijnÞ

T

D E

¼

jnfj

T n

D E

h

### v

ijn hfij

T

n ð4Þ

reﬂects the statistical dependence in directionn, which could be direction dependent. The statistical dependence has been investi-gated using the statistical dependence theory as detailed later in Section4. It will be shown based on the particle-scale information obtained from DEM that the statistical dependence between the contact vectors and contact forces is almost isotropic, i.e.,

jnfj T n

D E

¼

h

ijn hfij

T

(3)

where

### 1

is a direction independent scalar. It is hence taken as an assumption to avoid unnecessary complication. With this assump-tion, Eq.(3)can be rewritten as:

¼

N V

I

X

ecðnÞh

ij

n hfij

T

nd

### X

ð6Þ

In Eq.(6), there are scalar quantities including the coordination number

### x

, the particle density N=V, the statistical dependence coefﬁcient

### 1

and an integration over direction of the multiplication of the contact normal probability densityec(n), the mean contact vectorhvi|nand the mean contact forcehfi|n.

2.2. Contact normal probability density ec(n)

Orientations can be represented by direction vectors of unit length. For point contacts, each contact is associated with two con-tact normals, represented by unit normal vectorsnandn, respec-tively. The probability density of contact normals can be approximated by an even functionEc(n), symmetric with respect to directionn, i.e.,Ec(n) =Ec(n). WithEc

ðnÞbeing the probability density distribution, it must satisfy:

I

X

EcðnÞd

### X

¼1 andEcðnÞP0 ð7Þ

Using a polynomial in unit direction vectornwith

indetermi-nate coefﬁcients (Kanatani 1984; Li and Yu, 2011), then-th rank approximation takes the following form:

EcðnÞ ¼ 1

E0

Fci1i2inni1ni2 nin ð8Þ

whereE0=

H

XdX. In the two dimensional space,E0= 2

### p

and in the three dimensional space,E0= 4

### p

. The rank of the approximation re-fers to the highest rank of the power terms in the polynomial expansion. For symmetric distributions, the rank of approximation

in Eq.(8)should only be even numbers, and the direction tensor

Fci1i2in is a symmetric tensor, i.e.,F

c i1i2in ¼F

c

ði1i2inÞ, () over the sub-scripts designates the symmetrisation of the indices.Fci1i2in is

re-ferred to as the direction tensor for contact normal density.

Making an orthogonal decomposition, Eq.(8)can be expressed

equivalently as:

EcðnÞ ¼ 1

E0

D0þDci1i2ni1ni2þ þDci1i2inni1ni2 ninþ

h i

ð9Þ

Each term in Eq.(9)is independent from the others. In view of its symmetry,Dci1i2...;in should be also symmetric with respect to

sub-scriptsi1,i2,. . .in, i.e.,Dci1i2...;in¼D

c

ði1i2inÞ. Being an orthogonal

decom-position,Dc

i1i2in is deviatoric, i.e.,D

c

i1ikilindikil¼0.D

c

i1i2inis termed

as the deviatoric direction tensor for contact normal density. The direction tensorsFc

i1i2inandD

c

i1i2incan be calculated from the given

dataset of contact normals as elaborated inAppendix A1. More de-tails are available inLi and Yu (2011).

2.3. Mean contact vectorhvi|n

Vector is a more general form of directional data. For vector-valued directional data, we are interested in both their probabil-ity densprobabil-ity and their mean values in each direction. This applies to both the mean contact vectorhvi|nand the mean contact force hfi|n.

Here we approximate the directional distribution of mean vec-torhvi|n, (which is the mean of all the contact vectorsvassociated

with the same contact normal directionn) with a polynomial

ser-ies hvi|n as a linear combination of ni1ni2 nin. The n-th rank

approximation of the contact vectorhvi|ntakes the following com-pact form:

VjðnÞ ¼

### v

0Hvji1inni1ni2 nin ð10Þ

where

### v

0=HXhvi|nndX/E0is the directional average ofhvi|nn, i.e., the component ofhvi|ncoaxial withn. It is noted that for contact vectors the rank of the direction tensors is one order higher than that of approximation. Hvji

1in is a tensor symmetric with respect

to the subscriptsi1,i2,. . .in,. . .i.e.,Hvji1i2in ¼H

v

jði1i2inÞ, and is referred to as the direction tensor for mean contact vector. It characterizes the directional dependence of the mean contact vectorhvi|n.

Contact vectors are deﬁned as vectors pointing from the contact points to the particle centres. Noticing that under quasi-static con-dition, all the particles are in equilibrium. Eq.(1)holds true with the particle centre being a ﬁxed reference point for each particle. It is not necessarily to be the conventional choice as its centre of mass. If the particles have centre-point symmetric geometries, we could assume that the contact vectors are anti-symmetric with respect to direction n, i.e., hvi|n=hvi|n. The approximations

should hence have only terms of odd powers of n. Making an

orthogonal decomposition, the n-th rank approximation of hvi|n takes the following expansion form

VjðnÞ ¼

### v

0 njþGvji1ni1þ þG

v

ji1inni1 ninþ

h i

ð11Þ

in which Gvji

1in is deviatoric and symmetric with respect to the

subscriptsi1,i2,. . .in,. . .i.e.,Gvji1i2in¼G

v

jði1i2inÞ andG v

ji1ikilindikil¼0.

Gvji

1in is referred to as the deviatoric direction tensor for the mean

contact vector. The methods and procedures to calculate the direc-tion tensorsHvji

1inandG

v

ji1inbased on the given discrete dataset has

been carefully elaborated (Li and Yu, 2011). It is also briefed in

Appendix A2for completeness.

2.4. Mean contact forcehfi|n

According to Newton’s 3rd law of motion, there are a pair of ac-tion and reacac-tion forces at each contact point acting on the two bodies, respectively, which are of equal magnitudes and opposite directions. Hence, it is reasonable to assume the mean contact

force is an anti-symmetric function with respect to direction n,

i.e., hfi|n=hfi|n. Similarly to the method used to approximate the directional distribution for mean contact vectors, the contact forces averaged over contacts sharing the same normal directions can be approximated by following the compacted form as follows:

FjðnÞ ¼f0Hfji1i2inni1ni2 nin ð12Þ

or by following the form of an orthogonal decomposition as follows:

FjðnÞ ¼f0 njþGfji1ni1þ þGfji1inni1 ninþ

h i

ð13Þ

wheref0represents the directional average of mean normal contact force hfni|

n=hfi|nn, i.e., f0=

H

Xhfi|nndX/E0; Hfji1i2in andG

f ji1in are

the direction tensor and the deviatoric direction tensor for mean contact force, respectively.Gfji

1in is symmetric and deviatoric with

respect to subscripts i1,i2,. . .in,. . . i.e., Gfji1i2in ¼G

f

jði1i2inÞ and Gf

ji1ikilindikil¼0. The determination of the direction tensors from

discrete directional dataset follows the same methods and proce-dures as those described for mean contact vectors. They are not re-peated here due to space limitation.

2.5. General expressions for the stress–force–fabric relationship

(4)

Following the expressing given in Eqs.(8), (10), and (12), Eq.(6)

can be transformed as follows:

ij¼

N V

### v

0f0F

c k1knH

v il1lsH

f

jm1mtnk1 nknnl1 nlsnm1 nmt ð14Þ

where ¼HXðÞdX=E0denotes the average of⁄over directions. The identityni1ni2 ni2n1ni2nis a constant matrix. It has been derived in Li and Yu (2011)that:

ni1ni2 ni2n1ni2n¼

### a2nd

ði1i2di3i4 di2n1i2nÞ ð15Þ

where

### a

2n¼ 2nC

n

22n;D¼2

1 2nþ1;D¼3

(

, and dijis the Kronecker delta, and nCk

stands for the number ofk-combinations of an-element set. The stress tensor in Eq.(1)possesses all the properties of the

Cauchy stress tensor used in continuum mechanics

(Rothenburg and Selvadurai 1981). In the quasi-static condition, the moment equilibrium imposes the symmetry of the stress tensor, i.e.,

ij¼

### r

ji. Hence, the following equation should be satisﬁed:

Fk1knðH

v il1lsH

f jm1mtH

v jl1lsH

f

im1mtÞ nk1nknnl1nlsnm1nmt¼0: ð16Þ

By substituting the orthogonal decomposed expressions Eqs. (9),

(11), and (13)into Eq.(14), we have:

ij¼

V

### v

0f0 ninjþ

X/

t¼1

Gf

jm1mtninm1 nmtþ

X/

s¼1

Gvil1lsnjnl1nls

þX

/

s;t¼1

Gf jm1mtG

v

il1lsnl1nlsnm1nmt

þX

/

n¼2

Dc

k1knnk1nknninj

þ X

/

n¼2;t¼1

Dc k1knG

f

jm1mtnk1nknninm1nmt

þ X

/

n¼2;s¼1

Dc k1knG

v

il1lsnk1nknnl1 nlsnj

þ X

/

n¼2;s¼1;t¼1

Dck1knG

f jm1mtG

v

il1lsnk1nknnl1 nlsnm1nmt

2 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 5

ð17Þ

Being orthogonal decompositions, we have the coefﬁcient ten-sors satisfying

Dci1inni1ni2 ninnj1nj2 njm ¼0 Gvi0i1isni1ni2 nisnj1nj2 njt ¼0

Gfi0i1isni1ni2 nisnj1nj2 njt ¼0

ð18Þ

whenm<n,t<s,mandnare even numbers,sandtare odd numbers. Following the derivation inAppendix A3, Eq.(17)can be simpliﬁed as:

¼

N V

### v

0f0

ninjþG f

jm1ninm1þG

v

il1nl1njþDk1k2c nk1nk2ninj

þX

/

s¼1

Gfjm1msG v

il1lsnl1 nlsnm1 nms

þ X

/

n¼2;even

Dck1knG f

jm1mn1nink1 nknnm1 nmn1

þ X

/

n¼2;even

Dc

k1knG

f

jm1mnþ1nink1 nknnm1 nmnþ1

þ X

/

n¼2;even

Dck1knGvim1mn1njnk1 nknnm1 nmn1

þX

/

n¼2

Dc

k1knG

v

im1mnþ1njnk1 nknnm1 nmnþ1

þ X

/

n¼2;s;t¼1;jstj6n6sþt

Dc

k1knG

v

il1lsG

f

jm1mt

nk1 nknnl1 nlsnm1 nmt

2 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 5

ð19Þ

For any symmetric and deviatoric tensorDi1i2in, we have (Li and Yu, 2011):

Dj1j2jnnj1nj2 njnni1ni2 nin¼

### a2n

2n

2nC

n

Di1i2in ð20Þ

With this relationship, the terms in Eq.(19)can be calculated

indi-vidually as detailed inAppendix A4. And the stress tensor hence

becomes:

ij¼x

N V 1

### v

0f0

a2dijþa2Gfjiþa2G

v

ijþ23a4D c ijþ

X/

s¼1

a2s2s

2sCsG

f jl1lsG

v

il1ls

þX

/

n¼2

a2n2n

2nCnD

c im1mn1G

f jm1mn1þ

X/

n¼2

a2nþ2 2

nþ1 2nþ2Cn

þ1D c k1knG

f jik1kn

þX

/

n¼2

a2n2n

2nCnD

c im1mn1G

v

jm1mn1þ

X/

n¼2

a2nþ2 2

nþ1 2nþ2C

nþ1D c k1knG

v

jik1kn

þ X

/

n¼2;jstj6n6sþt

a2n2n

2nCnD

c k1knQ

vf;st ijk1kn

2 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 5

ð21Þ

This equation expresses the stress tensor in terms of direction ten-sors that characterize the internal structure (fabric) and inter-parti-cle reaction forces, and is referred to as the stress–force–fabric (SFF)

relationship, following the terminology proposed by Rothenburg

and Bathurst (1989).

3. Statistical features of granular materials

The expression of Eq.(21)is mathematically derived from the

micro-structural expression of the stress tensor as in Eq.(1). The only assumption we have adopted is the statistical dependence be-tween contact vectors and contact forces being isotropic. The rank of approximation can be very high. Experimental and numerical work in granular mechanics suggested that the directional distri-butions can be approximated with limited ranks of approximation (Oda et al., 1985; Rothenburg and Bathurst, 1989). In this section, we analyze the particle-scale information obtained from DEM. By conducting the directional statistical analyses, we could determine the rank of approximation based on the particle-scale directional data, and use the observations to simplify the general expression given as Eq.(21). With the particle scale information obtained from two dimensional numerical simulations, the analyses described in this section are limited to two dimensional cases.

Using the numerical experimental technique developed in Li

et al. (2013), the elementary behavior of two dimensional granular materials subjected to various loading paths have been simulated and reported (Li and Yu, 2009, 2010). In these numerical experi-ments, each particle is formed by clumping two equal-sized disks together. The distance between the centres of the two disks is equal to 1.5 times the disk radius,r. The particle size was uniformly distributed within the range (0.2, 0.6 mm) in terms of equivalent

diameter, and the disk thickness wast¼0.2 mm. The number of

particles used is about 3500, and according to Rothenburg and

Bathurst (1989)is sufﬁcient to model an inﬁnite system for

pur-poses of force balance in two dimensional assemblies.

The mechanical interaction between two elastic disks were de-rived based on the contact theories (Li, 2006) and used in the sim-ulations. In two dimensional cases, the contact law includes two linear elastic models (normal and tangential) of equal stiffnesses, and a slip model. The effect of contact moment is ignored. Both the normal and tangential particle stiffnesses were set to be 105N=m. The coefﬁcient of friction was

### l

(5)

An isotropic specimen was prepared using the radius expansion method, and then subjected to isotropic consolidation up to conﬁn-ing pressurepc¼1000 kPa before biaxial shearing. The void ratio

at Pc= 1000 kPa was 0.192. The specimen preparation method

Li et al. (2013). The material responses have been observed to be in qualitative agreement with laboratory observations, though not repeated here due to space limitation. During shearing, the ma-jor principal strain direction

### a

ewas ﬁxed, the mean normal stress was kept constant, while the magnitude of deviatoric strain

### e

qwas increasing. Loading applied vertically is denoted by angle 90, in terms of its deviation to thex1axis.

3.1. Contact normal density ec(n)

The directional distribution of contact normal density can be approximated using the compacted form of polynomial expansions as in Eq.(8)or in the form of orthogonal decomposition as in Eq.(9)

with its main statistical features reﬂected by the direction tensor

Fc

i1inor alternatively the deviatoric direction tensorD

c

i1in. The

lat-ter is used here since the deviatoric tensor can be delat-termined inde-pendently for different ranks of approximation.

In two dimensional spaces, a symmetric and deviatoric tensor

Dci1in only has two independent components. Denoting

Dc 1z}|{1 1

n1 ¼anandDc

2z}|{1 1

n1 ¼bn, we have the tensor components

ex-pressed as follows:

Dc

11122zﬄﬄ}|ﬄﬄ{ 2

k ¼

ð1Þk=2

an; whenkis even ð1Þðk1Þ=2bn; whenkis odd (

ð22Þ

Withdn¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2

nþb

2

n q

and tan/n¼bn=an, we havean¼dncos/nand bn¼dnsin/n. It is shown inAppendix A5that then-th rank power

term in the orthogonal decomposition of Eq.(9)can be expressed

as:

Dc

i1inni1ni2 nin¼ancosnhþbnsinnh¼d

c

ncosðnh/

c

nÞ ð23Þ

It is a cosine function with the period 2

### p=

n, the magnitudednand the phase angle/n=n. With Eqs.(9) and (23), the directional distri-bution of the contact normal probability densityEc(n) can be

ex-pressed as a summation over even numbersnas

EcðnÞ ¼ 1

E0 1þX

n

dcncos nh/ c n

" #

ð24Þ

Based on particle-scale information obtained from discrete ele-ment simulations, the direction tensors for contact normal density

Fci1inandD

c

i1inwere calculated following the procedure introduced

inAppendix A1. They were then used to determine the magnitudes

and phase angles in Eq. (24). The magnitudes of the 2nd, 4th and 6th rank orthogonal decompositions, dc2, dc4, dc6, are plotted in

Fig. 1(a). It is shown that the magnitude of deviatoric direction ten-sor decreases rapidly as the rank of approximation increases. The 2nd rank orthogonal decomposition is observed to be the main contributor to the direction dependent distribution of contact nor-mal density, while the 4th and 6th rank terms are negligible. As shear continues, the material fabric anisotropy gradually increases in order to withstand the external shearing. The phase angle of the 2nd rank approximation is/2=2 = 90

as shown inFig. 2(b), sug-gesting that the maximum probability density is co-directional with the loading direction. With the negligible magnitudes for the 4th and 6th rank terms, the values of their phase angles are of little signiﬁcance and hence not plotted in the ﬁgure.

In summary, the numerical observation indicates that the direc-tional distribution of the contact normal probability densityEc(n) can be sufﬁciently approximated by up to 2nd rank power terms as:

EcðhÞ ¼ 1 2

### p

1þd

c

2cos 2h/ c 2

ð25Þ

In terms of direction tensors, it is:

Dc

i1i2¼d

c 2

cos/c2 sin/ c 2 sin/c2 cos/

c 2

ð26Þ

3.2. Mean contact vectorhvi|n

The directional distributions of mean contact vector could be

approximated using the compacted form as in Eq.(10) or in the

form of orthogonal decomposition as in Eq.(11)with its main sta-tistical features reﬂective by the direction tensorHvji

1i2inor

alterna-tively the deviatoric direction tensorGvji1in. In analogy to Eq.(23),

then-th power term of Eq.(11)in two dimensional spaces could

be expressed as:

gvnj¼Gvji1inni1ni2 nin¼avnjcosnhþb v

njsinnh

¼dvnjcosðnh/vnjÞ ð27Þ

wheredvnjand/vnj=nstand for the magnitudes and phase angles for then-th rank orthogonal decomposition terms, respectively.

Denoting Avn¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dvn12þdvn222dvn1dvn2sinð/vn1/vn2Þ

q

=2, Bvn¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dvn21þd

v2

n2þ2d v n1d

v

n2sinð/vn1/vn2Þ

q

=2,

### a

v

n¼arctan d

v

n1sin/vn1

dvn2cos/vn2Þ= d v

n1cos/vn1þd v n2sin/vn2

, bvn¼arctan d

v

n1sin/vn1þ

dvn2cos/vn2Þ=dvn1cos/nv1dvn2sin/vn2, then-th power term becomes:

gvnj¼Gvji1inni1 nin¼A v n

cos nh

v n

sin nh

### a

v n

!

þBvn

cos nhbvn

sinnhbvn

!

ð28Þ

The expression suggests that then-th power term in Eq.(11)

can be decomposed into two components whose magnitudes being

Avn and Bvn, respectively. With Eqs.(11) and (28), the directional distribution of mean contact vectorhvi|nis expressed in terms of

summation taken over odd numbernas:

h

ijn¼

0 cosh

sinh 0 B @

1 C

AþX

n Avn

cos nh

v n

sinðnh

### a

v nÞ 0

B @

1 C

AþX

n Bvn

cosðnhbvnÞ

sinðnhbvnÞ

0 B @

1 C A 2

6 4

3 7 5

ð29Þ

The deviatoric direction tensorGv

jiz}|{1111

n1 is:

Gv

ji1111

zﬄﬄ}|ﬄﬄ{n1 ¼GvA ji1111

zﬄﬄ}|ﬄﬄ{n1 þGvB ji1111

zﬄﬄ}|ﬄﬄ{n1 ¼Avn cosav

n sinavn

sinav n cosavn

þBvn

cosbvn sinbvn

sinbvn cosbvn

ð30Þ

As shown in Appendix A2, we have Gjj¼Hjjdjj¼mD

0Kjjdjj¼0, indicatingAv1¼0.

With then-th power term of mean contact vector given in Eq.

(28), its normal componentgvn

n in the normal directionn= (cosh, -sinh) and its tangential componentgvt

n in the tangential direction t= (sinh, cosh) could be determined as:

gvn

n ¼gvnn¼Avncos ðn1Þh

### a

vn

þBvncos ðnþ1Þhbvn

ð31Þ

gvt

n ¼gvnt¼Avnsin ðn1Þh

vn

Bvnsin ðnþ1Þhbvn

ð32Þ

(6)

h

nij

0 1þ X

n

Avncos ðn1Þh

vn

þX

n

Bvncos ðnþ1Þhbvn

" #

ð33Þ

h

tij

0 X

n

Avnsin ðn1Þh

### a

vn

X

n

Bvnsin ðnþ1Þhbvn

" #

ð34Þ

They are summation of sinusoidal terms whose magnitudes areAvn

andBvn with the corresponding periods being 2

/(n1) and 2

### p

/ (n+ 1), and the corresponding phase angles being

### a

v

n=ðn1Þand

bvn=ðnþ1Þ.

With the pre-determined approximation for contact normal density, Hvji1i2in and G

v

ji1i2in were calculated from particle-scale

data following the procedure introduced in Appendix A2, and

then used to determine the magnitudes,Avn,Bvn, and phase angles,

### a

v

n, bvn in Eq. (28) accordingly. The magnitudes for 1st, 3rd, 5th rank termsAv1,Bv1,Av3,Bv3,Av5, Bv5, are plotted inFig. 2(a). Av10 is observed as expected. The anisotropy in the mean contact vec-tor is observed to be small, despite the non-circular particle shape used in the simulations. This may be due to the fact that the spec-imen starts with an almost isotropic distribution of particle

orien-tation. Upon shearing, Bv1 is observed to continuously increase

with the corresponding phase angle given inFig. 2(b). The phase

anglebv1=2 remains about 0, suggesting the preferred direction is

normal to the loading direction, as a result that as shearing con-tinues, the particle orientations tend to be normal to the loading direction.

Considering the possibility of non-circular particle shape and potential particle orientation anisotropy, 1st rank approximation is used to approximate the mean contact vector as:

h

ijn¼

### v

0

cosh sinh

þBv1

cosðhbv1Þ

sin hbv1

!

" #

ð35Þ

In the form of direction tensors, we have one termGvji

1as

Gvji1¼Bv1

cosbv1 sinbv1 sinbv1 cosbv1

ð36Þ

3.3. Mean contact forcehfi|n

The directional distributions of mean contact force can be

approximated using the compacted form as in Eq.(12)or in the

form of orthogonal decomposition as in Eq.(13)with its main sta-tistical features reﬂective by the direction tensorHf

ji1i2inor

alterna-tively the deviatoric direction tensorGf

ji1in. Then-th power term of

Eq.(13)in two dimensional spaces could be expressed as:

gf

nj¼G

f

ji1inni1ni2 nin¼afnjcosnhþb

f

njsinnh

¼dfnjcosðnh/

f

njÞ ð37Þ

(a) Magnitude (b) Phase angle

0 5 10 15 20 25

0 0.1 0.2 0.3 0.4 0.5 0.6

Deviatoric Strain εq(%)

A

n

is

otr

opic

M

agnitude

, dn

2nd rank, d2c 4th rank, d4c 6th rank, d6c

0 5 10 15 20 25

0 30 60 90 120 150 180

Deviatoric Strain εq(%)

P

h

as

e A

n

g

le,

φn c/n

(

o)

2nd rank, φ2c/2

Fig. 1.Approximation of contact normal density.

(a) Magnitude (b) Phase angle

0 5 10 15 20 25

0 0.02 0.04 0.06 0.08 0.1

Deviatoric Strain εq(%)

M

agnitude

1st rank, A

1

v 3rd rank, A 3

v 5th rank, A 5 v

1st rank, B

1

v 3rd rank, B 3

v 5th rank, B 5 v

0 5 10 15 20 25

-90 -60 -30 0 30 60 90

Deviatoric Strain εq(%)

P

h

as

e An

g

le (

o)

1st rank, βv 1/2

(7)

wheredfnjand/ f

nj=nstand for the magnitudes and phase angles for then-th rank orthogonal decomposition terms, respectively.

Denoting Afn¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dfn21þd

f2

n22d

f n1d

f n2sinð/

f n1/

f n2Þ

q

=2, Bfn¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ dfn21þd

f2

n2þ2d

f n1d

f n2sinð/

f n1/

f n2Þ

q

=2,

### a

f

n¼arctan dfn1sin/

f n1

h

dfn2cos/

f n2

= dfn1cos/

f n1þd

f n2sin/

f n2

i

, bfn¼arctan d f n1sin/

f n1þ

h

dfn2cos/

f n2

= dfn1cos/

f n1d

f n2sin/

f n2

i

, the n-th power term

becomes:

gfnj¼G f

ji1inni1 nin¼A

f n

cos nh

f n

sinðnh

### a

f

0 @

1 AþBfn

cosnhbfn

sinðnhbfnÞ

0 @

1 A

ð38Þ

The deviatoric direction tensorGf

ji1111z}|{

n1 is hence expressed as:

Gf

ji1111z}|{

n1 ¼G fA

jiz}|{1111

n1 þG fB

jiz}|{1111

n1

¼Afn

cos

f

n sin

fn

sin

f

n cos

### a

fn

0 B @

1 C AþBf

n

cosbfn sinb f n

sinbfn cosb f n 0 B @ 1 C A

ð39Þ

andAf1¼0. With Eqs.(13) and (39), the directional distribution of mean contact forcehfi|nis expressed in terms of summation taken

over odd numbernas:

hfijn¼f0

cosh sinh þX n Af n

cosðnh

f

sinðnh

### a

f

nÞ ! þX n Bf n

cosðnhbfnÞ

sinðnhbfnÞ

!

" #

ð40Þ

With then-th power term of mean contact force given in Eq.

(38), its normal componentgfnn and its tangential componentgftn could be expressed as:

gfn

n ¼g

f

nn¼A

f

ncos ðn1Þh

f n

þBfncos ðnþ1Þhb

f n

ð41Þ

gft

n¼gfnt¼A

f

nsin ðn1Þh

### a

fn

Bf

nsin ðnþ1Þhb

f n

ð42Þ

The approximation of the normal and tangential components of hfi|nwith up ton-th rank of approximation becomes:

hfnij

h¼f0 1þ X

n

Afncos ðn1Þh

### a

f n

þX

n

Bfncos ðnþ1Þhb f n

h i

" #

ð43Þ

hftij

h¼f0 X

n

Afnsin ðn1Þh

### a

fn

X

n Bf

nsin ðnþ1Þhb

f n

h i

" #

ð44Þ

They are summation of sinusoidal terms whose magnitudes areAf

n andBfn with the corresponding periods being 2

/(n1) and 2

### p

/ (n+ 1), and the corresponding phase angles being

### a

f

n=ðn1Þand

bfn=ðnþ1Þ.

With the approximation of directional distributed contact nor-mal density, the direction tensors for mean contact forceHfji

1i2in

andGf

ji1i2inwere calculated from particle-scale data, and were used

to determine the magnitudes, Afn, Bf

n, and phase angles,

### a

f n, bfn accordingly. The magnitudes for 1st, 3rd, 5th rank terms,Af1,B

f

1,

Af

3,B

f

3,A

f

5,B

f

5, are plotted inFig. 3(a). It is observed that the magni-tudes of orthogonal decomposition diminish quickly as the rank of approximation increases. Only terms relating toBf1,Af3are consid-ered to be signiﬁcant and other terms are negligible. Their

corre-sponding phase angles are given inFig. 3(b). Both phase angles

bf1=2 and

### a

f

The results indicate that the directional distribution of mean contact force hfi|n could be sufﬁciently approximated by up to 3rd rank of power terms as:

hfijn¼f0

cosh

sinh !

þBf1

cosðhbf1Þ

sinðhbf1Þ

0 @

1 AþAf3

cosð3h

f

sinð3h

### a

f

3Þ 0 @ 1 A 2 4 3 5

ð45Þ

In the form of direction tensors, we have two deviatoric direction tensorsGf

ji1andG f ji1i2i3as:

Gfji1¼B f 1

cosbf1 sinb f 1

sinbf1 cosb f 1 0

@

1

A; Gfji111¼A

f 3

cos

f

3 sin

f 3

sin

f

3 cos

### a

f 3 0 @ 1 A

ð46Þ

The rest component ofGf

ji1i2i3can be found easily as it is symmetric and deviatoric with respect toi1,i2,i3.

3.4. Simpliﬁcation based on the chosen limited ranks of approximation

In summary, statistical analyses based on micro-scale data for an isotropic specimen subjected to biaxial shearing suggest that it is sufﬁcient to approximate the directional distributions of contact normal density, mean contact forces and mean contact vectors with up to 2nd, 3rd and 1st ranks of power terms as given

in Eqs. (25), (35), and (45). These observations can be used to

simplify Eq. (21) by keeping only direction tensors of Dci1i2, G v ji1

andGfji1,G f ji1i2i3.

With the chosen ranks of approximation and Eq.(15), we have:

X/

n¼2;s;t¼1;jstj6n6sþt

Dck1knGvil1lsG f

jm1mtnk1 nknnl1 nlsnm1 nmt

¼Dc

k1k2G

v

il1G

f

jm1nk1nk2nl1nm1þDck1k2G

v

il1G

f

jm1m2m3nk1nk2nl1nm1nm2nm3

¼2

3

D

c

l1m1Gvil1G

f

jm1þ

### a4

22

4C2D c

k1k2Gv

f;13

ijk1k2

ð47Þ

Following Eqs.(A27) and (A28)inAppendix A4, we have

Gvil1G f

jm1m2m3nl1nm1nm2nm3np1np2¼

### a6

23

6C

3 Gvil1G

f

jl1p1p2 ð48Þ

Hence Eq.(21)can be simpliﬁed as:

¼

N V

0f0

ðdijþGf

jiþG

v

ijþG

f

jl1G

v

il1Þ

þ2

3

ðD

c

ijþD

c

im1G

f

jm1þD

c

im1G

v

jm1þD

c

l1m1G

v

il1G

f

jm1Þ

þ2

5

### a6

ðD

c

k1k2G

f

jik1k2þD

c

k1k2G

v

il1G

f jl1p1p2Þ 2 6 6 6 6 6 4 3 7 7 7 7 7 5

ð49Þ

Eq.(49)is valid for both two dimensional spaces and three dimen-sional spaces as long as the chosen ranks for approximation are con-sidered sufﬁcient.

3.5. Stress–force–fabric relationship in two dimensional spaces

In two dimensional spaces, Eq. (15) gives

2¼1=2;

4¼3=8;

(8)

¼

N 2V

### v

0f0

dijþGf

jiþG

v

ijþG

f jl1G v il1 þ1 2 D c

ijþD

c

ik1G

f

jk1þD

c

jk1Gvik1þD

c

k1k2Gvik1G

f jk2 þ1 4 D c

k1k2G

f

jik1k2þD

c

k1k2G

v

il1G

f jl1k1k2 2 6 6 6 6 4 3 7 7 7 7 5

ð50Þ

The expression can be further simpliﬁed by invoking the symmetry in the Cauchy stress tensor, i.e.,

12=

### r

21.Notice thatDci1i2,G

v ji1and

Gf

ji1 are symmetric and deviatoric tensors. With the expressions of direction tensorsDc

i1i2,G v ji1 andG

f ji1,G

f

ji1i2i3 given in Eqs.(26), (36),

and (46)respectively, we found that:

Gfjl1G v

il1¼B

f

1Bv1

cosðbf1Bv1Þ sin b f

1Bv1

sin bf1Bv1

cos bf1Bv1

0 B @ 1 C

A ð51Þ

Dcik1G f

jk1¼d

c

2B

f 1

cos /c2b f 1

sin /c2b

f 1

sin /c2b f 1

cos /c2b f 1 0 B @ 1 C

A ð52Þ

Dcjk1G v

ik1¼d

c

2Bv1

cos /c2bv1

sin /c2bv1

sin /c2bv1

cos /c2bv1

!

ð53Þ

Dc

k1k2G

f

jik1k2¼2d

c

2A

f 3

cos /c2

f 3

sinð/c2

f

sinð/c2

f

3Þ cosð/

c

2

f

0 @

1

A ð54Þ

Dck1k2Gvik1G f

jk2¼d

c

2Bv1B

f 1

cosð/c2bv1þb f

1Þ sinð/

c

2bv1þb

f

sinð/c2bv1þb f

1Þ cosð/

c

2bv1þb

f

!

ð55Þ

Dck1k2Gvil1G f

jl1k1k2¼2d

c

2Bv1A

f 3

cosð/c2þbv1

f

3Þ sinð/

c

2þbv1

f

sinð/c2þbv1

f

3Þ cosð/

c

2þbv1

### a

f

!

ð56Þ

The joint productsDck1k2G v ik1G

f jk2andD

c k1k2G

v il1G

f

jl1k1k2 are found to be

symmetric and deviatoric. However, Gf

jl1G v il1;D

c ik1G

f jk1;D

c jk1G

v ik1;

Dc k1k2G

f

jik1k2could be asymmetric if the eigenvectors ofD c i1i2,G

v ji1and

Gfji

1 are not co-incident. Since the stress tensor is to be symmetric, ½Gfjl

1G v il1þ

1 2ðD

c ik1G

f jk1þD

c jk1G

v ik1Þ þ

1 4D

c k1k2G

f

jik1k2 has to be symmetric. Hence,

Bf

1Bv1sinðb

f

1Bv1Þ

1

2 d c

2B

f

1sin /

c

2b

f 1

dc2Bv1sin /

c

2bv1

dc2A

f

3sin /

c

2

### a

f 3

h i

¼0:

As a result, we can write

Gfjl1G v il1þ 1 2 D c ik1G f

jk1þD

c

jk1Gvik1

þ1 4D c k1k2G f

jik1k2¼Cdij ð57Þ

where

C¼ B

f

1Bv1cosðb

f

1Bv1Þ þ12d

c

2B

f

1cosð/

c

2b

f

þ1

2d

c

2Bv1cosð/

c

2bv1Þ þ12d

c

2A

f

3cosð/

c

2

### a

f

" #

:

The stress tensor in Eq.(50)becomes:

¼

N

2V

### v

0f0 ð1þCÞdijþG f

jiþGvijþ

1 2D c ijþ 1 2D c

k1k2Gvik1G

f jk2 þ1 4D c

k1k2Gvil1G

f jl1k1k2

ð58Þ

The magnitudes of orthogonal decompositions are generally limited. The anisotropic magnitude in contact vectorGvji1has been observed to be small. The contribution from the two joint product terms,Dc

k1k2G v ik1G

f jk2andD

c k1k2G

v il1G

f

jl1k1k2, are expected to be extremely small, and hence negligible. This leads to a concise form of the stress–force–fabric relationship in two dimensional spaces as:

¼

N

2V

### v

0f0 ð1þCÞdijþG f

jiþG

v ijþ 1 2D c ij

ð59Þ

It is interesting to point out thatGfji

1i2i3do not appear directly in Eq.

(59). It contributes to and only to the coefﬁcientCthough the joint productDc

k1k2G f

jik1k2. In component form, we have:

¼xN

2V

### v

0f0 ð1þCÞ þ Bf1cos 2b f

1þBv1cos 2bv1þ12d c 2cos 2/

c 2

h i

¼

¼xN

2V

### v

0f0 B

f 1sin 2b

f

1þBv1sin 2bv1þ12d c 2sin 2/

c 2

h i

¼xN

2V

### v

0f0 ð1þCÞ B

f 1cos 2b

f

1þBv1cos 2bv1þ12d c 2cos 2/

c 2 h i 8 > > > > > > < > > > > > > :

ð60Þ

(a) Magnitude (b) Phase angle

0 5 10 15 20 25

0 0.1 0.2 0.3 0.4 0.5

Deviatoric Strain εq(%)

M

agnitude

1st rank, A

1

f 3rd rank, A 3

f 5th rank, A 5 f

1st rank, B

1

f 3rd rank, B 3

f 5th rank, B 5 f

0 5 10 15 20 25

0 30 60 90 120 150 180

Deviatoric Strain εq(%)

P h as e An g le ( o)

1st rank, βf

1/2 3rd rank, α f 3/2

(9)

WithDci1i2, G v ji1 andG

f

ji1 are symmetric and deviatoric tensors, we have the expression of the mean normal stress:

N

2V

ð1þCÞ

### v

0f0 ð61Þ

the normalized deviatoric stress tensor as:

¼

### rij

p dij¼

1 1þC G

f

jiþG

v

ijþ

1 2D

c ij

ð62Þ

The stress ratio is mainly determined byDcij,Gvij,G f

ji, and slightly af-fected byC. The principal stress direction could be predicted with

good conﬁdence based on the information on the magnitudesdc2,

Bf1,Bv1 and phases angles/c2,b

f

1,bv1. Among them, the anisotropic magnitudes from the ﬁrst two componentsdc2,Bf

1are observed to be much larger thanBv1, their inﬂuence is dominant.

3.6. The accuracy of the SFF relationship

With the pre-calculated direction tensors, the stress tensor can

be determined from Eq.(59). The accuracy of the derived stress–

force–fabric relationship was checked by comparing the prediction

from Eq.(59) and the stress measured directly on the specimen

boundary. The result is shown as inFig. 4in terms of the stress

invariantsp¼ ð

11þ

### r

22Þ=2,q¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

ð

11

22Þ2þ4

12

### r

21

q

and the principal stress directionha.

The coincidence of the two set of data conﬁrms that the derived stress–force–fabric relationship as deﬁned by Eq.(59)predicts the complete stress state with excellent accuracy. The main reason is that different from other physical models, the proposed stress– force–fabric (SFF) relationship has been mathematically derived by employing the directional statistical theory. Even though the expression of Eq.(59)seems very different from Eq.(1), they are equivalent as long as (1) the statistical dependence between the contact vectors and contact forces can be considered as isotropic; (2) it is sufﬁcient to approximate the directional distributions of contact normal density, mean contact forces and mean contact vectors with up to 2nd, 3rd and 1st ranks of power terms of direc-tion vectornas given in Eqs.(25), (35), and (45).

3.7. Comparison with Rothenburg and Bathurst’s SFF relationship (1989)

There is no doubt that even though the derivation process used

in this paper is different from that ofRothenburg and Bathurst

(1989), the resulted SFF relationships should be the same following

the same assumptions. The directional distributions used in

Roth-enburg and Bathurst (1989)are:

EcðhÞ ¼ 1

2p½1þaccos 2ðhhaÞ fnðhÞ ¼f

0½1þcncos 2ðhhaÞ

ftðhÞ ¼ f

0ctsin 2ðhhaÞ 8

> < >

: ð63Þ

The mean contact vector was assumed to be isotropic.

By keeping only terms ofBf1 andAf3in Eqs.(43) and (44), the normal and tangential components of mean contact forces become:

hfnij

h¼f0 1þBf1cosð2hb f

1Þ þA

f

3cosð2h

### a

f

h i

ð64Þ

hftij

h¼f0 Bf1sinð2hb f

1Þ þA

f

3sinð2h

### a

f

h i

ð65Þ

With the assumption of /c2¼b

f

### a

f

3¼2ha, and denoting

cn¼ ðBf1þA

f

3Þ,ct¼ ðBf1A

f

3Þ,d

c

2¼ac, the expressions given as Eqs.

(25), (64), and (65) become the same as Eq. (63), and the

coefﬁcientC¼ ½1 2d

c

2B

f

1þ12d

c

2A

f

3 ¼12accn. The stress–force–fabric rela-tionship given in Eq.(59)becomes:

¼

N

2V

### v

0f0 1þ

1 2accn

dijþ1

2ðacþcnþctÞ

cosha sinha sinha cosha

ð66Þ

The general stress–force–fabric relationship Eq.(59)developed in

this paper reduces to the special form given in Rothenburg and

Bathurst (1989) with the assumptions of /c2¼bf1¼

### a

f

3¼2ha and the contact vector distribution being isotropicGvij¼0.

4. Statistical dependence between contact vectors and contact forces

Section 2.1 assumed an isotropic statistical dependence

be-tween contact vectors and contact forces, i.e., h

jnfj

T ni ¼

h

### v

ijn hfij

T

n. Here, we will show how the assumption has been

sup-ported by statistical analyses based on the particle-scale

informa-tion. The statistical dependence can be investigated by

comparing the directional distribution ofh

ifji|n,h

### v

ii|nhfji|n.

4.1. Directional distribution ofh

### v

ifji|n

The method and procedure proposed byLi and Yu (2011)was

generalized to study direction dependent, multi-dimensional ar-rays, such ash

ifji|nandh

### v

ii|nhfji|n, as elaborated in the following. Taking the average of producth

### v

ifji|nas an even function with

re-0 5 10 15 20 25

0 200 400 600 800 1000 1200

Deviatoric Strain εq(%)

St

re

s

s

i

n

v

a

ri

a

n

ts

(k

Pa

)

p from Eq. (59) p Measurement q from Eq. (59) q Measurement

0 5 10 15 20 25

0 20 40 60 80 100 120

Deviatoric Strain εq(%)

P

ri

n

ci

p

a

l S

tr

e

ss D

ir

e

ct

io

n

,

θa

(

o)

From Eq. (59) Measurement

(10)

spect to directionn, then-th rank approximation ofh

### v

ifji|ntakes the compact form (nis an even integer):

ðViFjÞðnÞ ¼ ð

### v

fÞpa0P

pa

ijk1k2knnk1nk2 nkn ð67Þ

wherePpa

ijk1kn stands for the direction tensor. It is symmetric with

respect to subscriptsk1,k2,. . .kn, i.e.,Ppaijk1k2kn¼P

pa

ijðk1k2knÞ. The super-script suggests the sequence of operations. h

### v

ifji|nis obtained by ﬁrstly taking the tensor product of contact vectors and contact forces and then taking the average.ð

### v

fÞpa0 represents the directional average of dot producthvTfi|

n, i.e.,ð

fÞpa0 ¼

H Xh

### v

Tfij

ndX=E0. In the form of orthogonal decomposition, we have:

ðViFjÞðnÞ ¼ ð

### v

fÞpa0

dij DþQ

pa ij þQ

pa

ijk1k2nk1nk2þ þQ pa

ijk1knnk1 nknþ

ð68Þ

in whichQpaijk

1k2kn is the deviatoric direction tensor. It is symmetric

and deviatoric with respect to subscriptsk1,k2,. . .kn, i.e.,Qpaijk1k2kn¼

Qpa

ijðk1k2knÞ and Q pa

ijk1kkklkndkkkl¼0. The method to calculate the

direction tensors are given asAppendix A6.

4.2. Directional distribution ofh

ii|nhfji|n

h

### v

ii|nhfji|ncan be calculated by taking multiplication of Eqs. (11) and (13). Alternatively, we could apply a similar method and pro-cedure as detailed in Section4.1. The approximation can take the following compact form:

hViiðnÞhFjiðnÞ ¼ ð

### v

fÞap0P

ap

ijk1k2knnk1nk2 nkn ð69Þ

where the direction tensorPap

ijk1knis symmetric with respect to

sub-scriptsk1,k2,. . .kn, i.e.,Papijk1k2kn¼P

ap

ijðk1k2knÞ. Here what to be investi-gated ish

### v

ii|nhfji|n. It is obtained by ﬁrstly taking the averages of contact vectors and contact forces respectively and then multiply-ing them to get the product. Hence, we use the superscripts asap. ð

### v

fÞap0 represents the directional average of dot producthvi|nThfi|n, i.e., ð

fÞap0 ¼

H Xh

### v

ij

T

n hfijn dX=E0. In the form of an orthogonal decomposition, we have:

hViiðnÞhFjiðnÞ ¼ ð

### v

ap 0

dij

DþQ ap

ij þQ

ap

ijk1k2nk1nk2þ þQ

ap

ijk1knnk1 nknþ

ð70Þ

in which the deviatoric direction tensorQapijk

1k2kn is symmetric and

deviatoric with respect to subscripts k1,k2,. . .kn, i.e., Qapijk1k2kn¼

Qapijðk

1k2knÞ and Q ap

ijk1kkklkndkkkl¼0. The method to determine the

direction tensors is the same as that in Section4.1, hence is not repeated.

4.3. Observations on the statistical dependence

The statistical dependence between contact vectors and contact forces can be studied by comparing the direction distributions of h

ifji|n and h

### v

ii|nhfji|n. With the two distributions approximated with polynomial expansions as in Eqs.(68) and (70), the two direc-tional dependent multi-dimensional arraysh

ifji|nand h

### v

ii|nhfji|n can be compared in terms of their directional averages and their direction tensors of different ranks.

The directional averages and the 0th-rank deviatoric direction tensors for approximatingh

ifji|nandh

### v

ii|nhfji|nare calculated from particle-scale information following the procedure introduced in

Appendix A6and plotted inFig. 5. The value of

### v

0f0is also given in Fig. 5(a) as a reference value. The difference between ð

fÞpa0 andð

### v

fÞap0 shown inFig. 5(a) suggests that statistical dependence between contact vectors and contact forces does exist.ð

### v

fÞap0 is ob-served to be close to

### v

0f0as seen from the ﬁgure, indicating the contribution from joint product of higher rank anisotropic terms being negligible. The ratio ofð

fÞpa0=ð

### v

ap

0 has also been plotted

in the ﬁgure. It varies from 1.07 at beginning and decrease slightly to 1.04 at large strain levels.

The components of the deviatoric direction tensorsQpaij andQapij

are given inFig. 5(b). They are observed to be almost identical, indicating that the statistical dependence can be considered to be the same in different directions. Statistical analyses show that the magnitude of direction tensors decreases as the rank of approx-imation increases. Hence, higher rank approxapprox-imation would be ex-pected to be even less signiﬁcant. This observation supports the assumption made in Section2.1that the statistical dependence be-tween the contact vectors and contact forces is isotropic.

Analyses have been carried out on different specimens undergo-ing various loadundergo-ing paths. The isotropy in statistical dependence has been found as a generally valid assumption. In cases that sta-tistical dependence is shown to be strongly direction dependent, the SFF relationship can be established using similar procedure only that higher rank terms are to be introduced to reﬂect its direc-tional dependence and the results are expected to include some additional direction tensors.

Rothenburg and Bathurst (1989)’s SFF relationship is based on

the assumption that the principal directions of contact normal density, normal tangential contact force and tangential contact

(a) Directional averages (b) Deviatoric direction tensor

0 5 10 15 20 25

1 1.2 1.4 1.6 1.8 2

Deviatoric Strain εq(%)

Di

re

ct

io

n

al

av

er

ag

e (

1

0

-5m.

N

)

0 5 10 15 20 25

1 1.04 1.08 1.12 1.16 1.2

Ra

ti

o

(vf)pa0 (vf)ap0 v0f0 (vf)pa0/(vf)ap0

0 5 10 15 20 25

-0.2 -0.15 -0.1 -0.05 0 0.05 0.1 0.15 0.2

Deviatoric Strain εq(%)

De

vi

at

or

ic

di

re

ct

ion t

ens

or

Qpa11

Qap11

Qpa

12

Qap12

Qpa

21

Qap21

Qpa22

Qap

22

(11)

force are coaxial with the principal stress direction. It gives a good prediction in the mean normal stress and the stress ratio for ini-tially isotropic specimen subjected to proportional loading. How-ever, the coaxial assumption excludes the ability of predicting principal stress directions. Moreover, in non-proportional loading, the fabric and particle interaction may not always be co-axial (Li and Yu, 2009; Li and Yu, 2011). By characterizing the directional distributions in terms of direction tensor, the coaxial assumption

is not needed. Hence, Eq. (59) is applicable in non-proportional

Material behavior to non-proportional loading, involving rota-tion of either material fabric or principal stresses, has attracted

much research interest over the last few decades (Arthur et al.,

1980; Towhata and Ishihara, 1985; Gutierrez et al., 1991; Yoshi-mine et al., 1998; Li and Dafalias, 2004; Tsutsumi and Hashiguchi,

2005; Yu and Yuan, 2006; Yu, 2008).

In the effort to study the dependence of granular material behavior on initial fabric and loading paths,Li and Yu (2009) pre-pared two anisotropic specimens and sheared the specimens in dif-ferent directions to study material anisotropy. One was prepared using the deposition method, and was referred as the initially anisotropic specimen. The other was the preloaded specimen, pre-pared by shearing initially anisotropic specimen monotonically up to 25% axial strain in the deposition direction, and then unloaded to isotropic stress state. The two specimens were consolidated to

Noticeable difference in non-coaxiality with and without pre-shearing was reported (Li and Yu, 2009). Later, numerical simula-tion of stress rotasimula-tion has been reported (Li and Yu, 2010). The iso-tropic specimen was ﬁrstly sheared in the vertical direction

### a

r¼90

up to stress ratio

### g

¼0:8 and then subjected to pure stress rotation with continuous rotation of principal stress direction

### a

r. These two tests involved non-coincidence between the principal fabric direction, the principal stress directions and their relative rotations. Both are non-proportional loadings.

The data from these simulations were used here for statistical analyses. Directional statistical analyses conﬁrmed that even for non-proportional loadings the previous observations still hold true. That is to say, the magnitudes of orthogonal decomposition dimin-ish quickly as the rank of approximation increases. The 2nd rank approximation of contact normal densitydc2, the 1st rank and 3rd rank approximation of contact force,Bf1 andAf3, and the 1st rank approximation of contact vector,Bv1were all the anisotropic terms necessary to give sufﬁcient approximations. The 4th rank terms for contact normal densitydc4was observed to increase gradually as shear continues, while remain limited.

5.2.1. Anisotropic specimen subjected to monotonic shearing

For the anisotropic specimens subjected to monotonic shearing, results on the specimens when subjected to ﬁxed loading direction

### a

e¼30

were analyzed and presented here.

### a

edenotes the

Figs. 6 and 7give the magnitudes and phase angles for the ini-tially anisotropic specimen and the preloaded specimen, respec-tively. Initially, the magnitude of contact normal dc2 was about 0.22. The phase angle of contact normal/c2=2 was 90, suggesting that the initial anisotropic structure had the preferred direction the same as particle deposition. As shear continued, its magnitude increased. In the meantime, its phase angle/c2=2 approached 30, coaxial with the loading direction.

5.2.2. Isotropic specimen to stress rotation

The statistical characteristics of the isotropic specimen sub-jected to stress rotation were plotted inFig. 8. The anisotropy in mean contact vector was observed to be negligible, while the anisotropy in contact normal density and contact forces were sig-niﬁcant. The phase angle of the 2nd rank contact normal density

/c2=2, and those of contact forces,bf1=2 and

### a

f

3=2 were plotted in Fig. 8(b). It was shown that the phase angles rotated together with the rotation of the principal stress direction. Again, the non-coax-iality between the contact normal density and the contact forces was noticeable. The differences between the phase angles were plotted inFig. 9. The 1st rank phase anglebf1=2 was observed al-most coincident with the principal stress direction, while the phase angles for the contact normal density/c2=2 and the phase angle for the 3rd rank contact force

### a

f

3=2 were left behind in the range of

10 20.

The comparisons of the stress tensor calculated from Eq.(59)

and those measured on the specimen boundary were given in

anisotropic specimens to monotonic loading and the isotropic specimen to stress rotation, respectively. The almost identical

re-sults conﬁrmed the capability of Eq. (59) to provide complete

and accurate prediction on the specimen stress state. The main reason is that the derivation of SFF relationship involved neither pre-assumption on the loading path nor material constitutive relationship. It is a mathematical approach. Eq.(59)provides good prediction on the material stress as long as the conditions of isotro-pic statistical dependence and the chosen ranks of approximation remain valid.

6. Beneﬁts of using directional statistical theories

This paper concerned about the same problem as inRothenburg